#------------------------------------------------------------------------------
#$Date: 2015-10-09 14:36:09 +0300 (Fri, 09 Oct 2015) $
#$Revision: 161812 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/58/7035857.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7035857
loop_
_publ_author_name
'Hu, Yang-Yang'
'Xiao-Zhang, ?'
'Zhao, De-Chuan'
'Guo, Hai-Yang'
'Fu, Li-Wei'
'Guo, Lan-Lan'
'Cui, Xiao-Bing'
'Huo, Qi-Sheng'
'Xu, Ji-Qing'
_publ_section_title
;
 Tuning the structures based on polyoxometalates from 1-D to 2-D by using
 different secondary organic ligands.
;
_journal_issue                   33
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              14830
_journal_page_last               14841
_journal_paper_doi               10.1039/c5dt02060c
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'C32 H36 Cu Mo12 N10 O44 Si'
_chemical_formula_weight         2507.62
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2015-07-14 deposited with the CCDC.
2015-07-17 downloaded from the CCDC.
;
_cell_angle_alpha                110.302(2)
_cell_angle_beta                 98.157(2)
_cell_angle_gamma                111.880(2)
_cell_formula_units_Z            1
_cell_length_a                   11.1938(13)
_cell_length_b                   12.7022(14)
_cell_length_c                   13.1616(15)
_cell_measurement_reflns_used    4167
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.29
_cell_measurement_theta_min      2.59
_cell_volume                     1547.6(3)
_computing_data_collection       'Bruker SMART'
_computing_molecular_graphics    'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0245
_diffrn_reflns_av_unetI/netI     0.0436
_diffrn_reflns_laue_measured_fraction_full 0.993
_diffrn_reflns_laue_measured_fraction_max 0.993
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            7773
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.993
_diffrn_reflns_theta_full        24.999
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_min         1.736
_exptl_absorpt_coefficient_mu    2.811
_exptl_absorpt_correction_T_max  0.561
_exptl_absorpt_correction_T_min  0.432
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            dark_green
_exptl_crystal_density_diffrn    2.691
_exptl_crystal_description       block
_exptl_crystal_F_000             1197
_exptl_crystal_size_max          0.330
_exptl_crystal_size_mid          0.300
_exptl_crystal_size_min          0.240
_refine_diff_density_max         1.734
_refine_diff_density_min         -1.406
_refine_diff_density_rms         0.336
_refine_ls_extinction_coef       0.0054(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.051
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     473
_refine_ls_number_reflns         5412
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.053
_refine_ls_R_factor_all          0.0983
_refine_ls_R_factor_gt           0.0876
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0604P)²+65.1497P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2099
_refine_ls_wR_factor_ref         0.2250
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4723
_reflns_number_total             5412
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c5dt02060c2.cif
_cod_data_source_block           shelx_3
_cod_depositor_comments
'Adding full bibliography for 7035855--7035860.cif.'
_cod_database_code               7035857
_shelx_shelxl_version_number     2014/7
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.457
_shelx_estimated_absorpt_t_max   0.552
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Mo1 Mo -0.31292(14) -0.14848(15) -0.21714(11) 0.0455(4) Uani 1 1 d . . .
Mo2 Mo -0.02094(18) 0.07165(14) -0.23619(11) 0.0510(5) Uani 1 1 d . . .
Mo3 Mo -0.29456(14) -0.20535(14) 0.02817(14) 0.0474(4) Uani 1 1 d . . .
Mo4 Mo -0.04652(18) -0.22433(16) -0.26983(11) 0.0574(5) Uani 1 1 d . . .
Mo5 Mo -0.25633(16) 0.09126(18) 0.04771(15) 0.0582(5) Uani 1 1 d . . .
Mo6 Mo 0.04909(19) 0.30467(15) 0.03994(16) 0.0605(5) Uani 1 1 d . . .
Cu1 Cu 0.0000 -0.5000 -0.5000 0.0430(7) Uani 1 2 d S . P
Si1 Si 0.0000 0.0000 0.0000 0.0320(12) Uani 1 2 d S . P
O1 O -0.0749(18) -0.0517(16) -0.1314(15) 0.027(4) Uani 0.5 1 d . . P
O2 O -0.1603(19) -0.0565(16) -0.0335(14) 0.030(4) Uani 0.5 1 d . . P
O3 O 0.0647(19) 0.1036(16) -0.0488(13) 0.028(4) Uani 0.5 1 d . . P
O4 O 0.0327(18) -0.1222(15) -0.0725(14) 0.025(4) Uani 0.5 1 d . . P
O5 O -0.4576(13) -0.2129(13) -0.3211(12) 0.075(4) Uani 1 1 d . . .
O6 O -0.2315(15) -0.2457(11) -0.2895(15) 0.080(5) Uani 1 1 d . . .
O7 O -0.3768(14) 0.1295(14) 0.0731(12) 0.067(4) Uani 1 1 d . . .
O8 O 0.0756(13) 0.4473(12) 0.0561(12) 0.061(3) Uani 1 1 d . . .
O9 O -0.0754(13) -0.3317(12) -0.3985(10) 0.059(3) Uani 1 1 d . . .
O10 O -0.0231(15) 0.1044(17) -0.3483(12) 0.081(5) Uani 1 1 d . . .
O11 O -0.0125(14) 0.2145(14) -0.1254(12) 0.085(5) Uani 1 1 d . . .
O12 O 0.0921(14) 0.329(2) 0.1913(15) 0.132(9) Uani 1 1 d . . .
O13 O -0.3161(18) -0.0596(13) 0.0703(10) 0.075(5) Uani 1 1 d . . .
O14 O 0.2199(16) 0.3175(16) 0.0365(13) 0.098(6) Uani 1 1 d . . .
O15 O -0.2019(16) -0.0209(12) -0.2620(16) 0.090(6) Uani 1 1 d . . .
O16 O -0.3286(19) -0.0113(13) -0.1103(11) 0.081(5) Uani 1 1 d . . .
O17 O -0.1799(16) -0.1499(15) 0.1724(14) 0.102(7) Uani 1 1 d . . .
O18 O -0.4370(14) -0.3045(14) 0.0334(11) 0.075(4) Uani 1 1 d . . .
O19 O 0.1362(15) -0.173(2) -0.2039(16) 0.133(10) Uani 1 1 d . . .
O20 O -0.3607(18) -0.2358(14) -0.1318(11) 0.075(5) Uani 1 1 d . . .
O21 O -0.0083(16) -0.0831(12) -0.2998(16) 0.084(5) Uani 1 1 d . . .
O22 O -0.1400(18) 0.2314(17) 0.0265(14) 0.094(5) Uani 1 1 d . U .
O23 O -0.1993(13) -0.6876(13) -0.3459(12) 0.070(4) Uani 1 1 d . . .
O24 O -0.1508(12) -0.6149(11) -0.4745(10) 0.053(3) Uani 1 1 d . . .
N1 N 0.1047(13) -0.4810(12) -0.3579(11) 0.041(3) Uani 1 1 d . . .
C6 C -0.1200(17) -0.6245(15) -0.3810(13) 0.044(4) Uani 1 1 d . . .
C15 C -0.542(2) -0.1500(17) -0.6252(14) 0.050(4) Uani 1 1 d . . .
H15A H -0.6141 -0.2086 -0.6158 0.060 Uiso 1 1 calc R U .
C14 C -0.421(3) -0.087(2) -0.5466(17) 0.066(6) Uani 1 1 d . . .
H14A H -0.4107 -0.1028 -0.4829 0.079 Uiso 1 1 calc R U .
N2 N 0.370(3) 0.3297(18) -0.2743(14) 0.086(6) Uani 1 1 d . . .
C5 C 0.0260(17) -0.5506(13) -0.3125(13) 0.041(4) Uani 1 1 d . . .
C13 C -0.312(3) -0.001(3) -0.555(2) 0.090(8) Uani 1 1 d . . .
H13A H -0.2296 0.0435 -0.4974 0.108 Uiso 1 1 calc R U .
C11 C 0.312(2) 0.304(2) -0.3841(17) 0.064(5) Uani 1 1 d . . .
C4 C 0.0816(19) -0.5567(16) -0.2128(15) 0.050(4) Uani 1 1 d . . .
H4A H 0.0282 -0.6086 -0.1848 0.060 Uiso 1 1 calc R U .
C1 C 0.2391(17) -0.4104(15) -0.3015(15) 0.050(4) Uani 1 1 d . . .
H1A H 0.2917 -0.3592 -0.3304 0.060 Uiso 1 1 calc R U .
C10 C 0.383(2) 0.348(2) -0.4470(15) 0.062(5) Uani 1 1 d . . .
H10A H 0.3383 0.3292 -0.5209 0.075 Uiso 1 1 calc R U .
N3 N 0.180(2) 0.226(2) -0.4323(18) 0.092(6) Uani 1 1 d . . .
H3B H 0.1413 0.2049 -0.5026 0.110 Uiso 1 1 calc R U .
H3C H 0.1328 0.1971 -0.3933 0.110 Uiso 1 1 calc R U .
C16 C -0.559(2) -0.130(2) -0.7138(18) 0.065(5) Uani 1 1 d . . .
N4 N -0.457(2) -0.041(2) -0.731(2) 0.097(7) Uani 1 1 d . . .
C3 C 0.221(2) -0.481(2) -0.1580(16) 0.062(5) Uani 1 1 d . . .
H3A H 0.2616 -0.4769 -0.0892 0.074 Uiso 1 1 calc R U .
C9 C 0.517(3) 0.419(2) -0.405(3) 0.104(9) Uani 1 1 d . . .
H9A H 0.5663 0.4432 -0.4513 0.125 Uiso 1 1 calc R U .
N5 N -0.690(2) -0.202(2) -0.795(2) 0.102(8) Uani 1 1 d . . .
H5A H -0.7536 -0.2562 -0.7829 0.122 Uiso 1 1 calc R U .
H5B H -0.7065 -0.1922 -0.8556 0.122 Uiso 1 1 calc R U .
C2 C 0.2992(18) -0.4103(17) -0.2082(17) 0.057(5) Uani 1 1 d . . .
H2A H 0.3928 -0.3641 -0.1754 0.069 Uiso 1 1 calc R U .
C12 C -0.329(3) 0.021(2) -0.657(3) 0.097(9) Uani 1 1 d . . .
H12A H -0.2561 0.0738 -0.6708 0.117 Uiso 1 1 calc R U .
C8 C 0.582(3) 0.456(2) -0.294(2) 0.087(7) Uani 1 1 d . . .
H8A H 0.6751 0.5086 -0.2632 0.104 Uiso 1 1 calc R U .
C7 C 0.511(3) 0.414(2) -0.2286(18) 0.093(9) Uani 1 1 d . . .
H7A H 0.5548 0.4417 -0.1522 0.111 Uiso 1 1 calc R U .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O5 Mo1 O20 102.3(7) . .
O5 Mo1 O6 99.7(8) . .
O20 Mo1 O6 92.6(6) . .
O5 Mo1 O16 100.0(8) . .
O20 Mo1 O16 89.8(5) . .
O6 Mo1 O16 159.1(8) . .
O5 Mo1 O15 98.2(8) . .
O20 Mo1 O15 159.4(8) . .
O6 Mo1 O15 86.3(6) . .
O16 Mo1 O15 84.2(6) . .
O5 Mo1 O2 160.2(8) . .
O20 Mo1 O2 64.9(7) . .
O6 Mo1 O2 96.0(7) . .
O16 Mo1 O2 66.4(7) . .
O15 Mo1 O2 94.8(7) . .
O5 Mo1 O1 156.8(7) . .
O20 Mo1 O1 97.4(7) . .
O6 Mo1 O1 66.9(6) . .
O16 Mo1 O1 92.2(7) . .
O15 Mo1 O1 63.3(7) . .
O2 Mo1 O1 42.6(6) . .
O10 Mo2 O15 101.6(8) . .
O10 Mo2 O11 102.3(8) . .
O15 Mo2 O11 93.0(6) . .
O10 Mo2 O21 98.7(8) . .
O15 Mo2 O21 88.7(6) . .
O11 Mo2 O21 158.2(8) . .
O10 Mo2 O17 96.2(8) . 2
O15 Mo2 O17 161.7(9) . 2
O11 Mo2 O17 87.2(6) . 2
O21 Mo2 O17 84.5(6) . 2
O10 Mo2 O3 156.2(7) . .
O15 Mo2 O3 99.7(8) . .
O11 Mo2 O3 65.9(6) . .
O21 Mo2 O3 92.3(7) . .
O17 Mo2 O3 63.8(8) 2 .
O10 Mo2 O1 158.5(7) . .
O15 Mo2 O1 64.5(7) . .
O11 Mo2 O1 95.1(7) . .
O21 Mo2 O1 66.1(6) . .
O17 Mo2 O1 97.3(8) 2 .
O3 Mo2 O1 44.6(6) . .
O18 Mo3 O13 101.2(8) . .
O18 Mo3 O17 100.4(8) . .
O13 Mo3 O17 92.7(6) . .
O18 Mo3 O14 100.7(9) . 2
O13 Mo3 O14 157.0(8) . 2
O17 Mo3 O14 90.2(6) . 2
O18 Mo3 O20 97.7(7) . .
O13 Mo3 O20 87.1(5) . .
O17 Mo3 O20 161.7(8) . .
O14 Mo3 O20 83.1(6) 2 .
O18 Mo3 O3 159.6(7) . 2
O13 Mo3 O3 94.7(7) . 2
O17 Mo3 O3 65.9(8) . 2
O14 Mo3 O3 65.9(7) 2 2
O20 Mo3 O3 95.8(6) . 2
O18 Mo3 O2 155.1(7) . .
O13 Mo3 O2 65.8(6) . .
O17 Mo3 O2 101.4(8) . .
O14 Mo3 O2 91.3(8) 2 .
O20 Mo3 O2 61.9(6) . .
O3 Mo3 O2 44.9(6) 2 .
O9 Mo4 O19 100.8(9) . .
O9 Mo4 O21 99.8(7) . .
O19 Mo4 O21 92.5(8) . .
O9 Mo4 O12 100.2(9) . 2
O19 Mo4 O12 89.2(6) . 2
O21 Mo4 O12 159.2(9) . 2
O9 Mo4 O6 97.1(7) . .
O19 Mo4 O6 161.9(9) . .
O21 Mo4 O6 87.2(6) . .
O12 Mo4 O6 84.8(7) 2 .
O9 Mo4 O4 156.6(6) . .
O19 Mo4 O4 64.3(8) . .
O21 Mo4 O4 98.8(7) . .
O12 Mo4 O4 63.4(8) 2 .
O6 Mo4 O4 97.8(7) . .
O9 Mo4 O1 154.7(6) . .
O19 Mo4 O1 99.9(9) . .
O21 Mo4 O1 64.8(6) . .
O12 Mo4 O1 94.4(9) 2 .
O6 Mo4 O1 63.7(6) . .
O4 Mo4 O1 48.3(6) . .
O7 Mo5 O16 101.3(7) . .
O7 Mo5 O22 101.0(8) . .
O16 Mo5 O22 91.8(7) . .
O7 Mo5 O13 99.3(7) . .
O16 Mo5 O13 88.3(5) . .
O22 Mo5 O13 159.2(8) . .
O7 Mo5 O19 98.7(9) . 2
O16 Mo5 O19 159.6(9) . 2
O22 Mo5 O19 88.0(7) . 2
O13 Mo5 O19 84.8(7) . 2
O7 Mo5 O4 155.8(7) . 2
O16 Mo5 O4 98.8(7) . 2
O22 Mo5 O4 65.0(7) . 2
O13 Mo5 O4 94.4(6) . 2
O19 Mo5 O4 62.7(8) 2 2
O7 Mo5 O2 155.3(7) . .
O16 Mo5 O2 63.3(6) . .
O22 Mo5 O2 98.7(7) . .
O13 Mo5 O2 62.9(6) . .
O19 Mo5 O2 96.5(9) 2 .
O4 Mo5 O2 48.4(6) 2 .
O8 Mo6 O14 99.3(7) . .
O8 Mo6 O12 101.5(9) . .
O14 Mo6 O12 90.2(8) . .
O8 Mo6 O22 100.3(7) . .
O14 Mo6 O22 160.1(8) . .
O12 Mo6 O22 89.6(7) . .
O8 Mo6 O11 100.5(7) . .
O14 Mo6 O11 87.7(6) . .
O12 Mo6 O11 157.9(9) . .
O22 Mo6 O11 85.0(7) . .
O8 Mo6 O4 156.7(6) . 2
O14 Mo6 O4 98.1(8) . 2
O12 Mo6 O4 62.9(8) . 2
O22 Mo6 O4 64.3(7) . 2
O11 Mo6 O4 95.7(7) . 2
O8 Mo6 O3 153.5(7) . .
O14 Mo6 O3 62.9(7) . .
O12 Mo6 O3 98.1(9) . .
O22 Mo6 O3 97.4(7) . .
O11 Mo6 O3 61.6(6) . .
O4 Mo6 O3 49.8(6) 2 .
O24 Cu1 O24 180.0 2_544 .
O24 Cu1 N1 96.0(5) 2_544 .
O24 Cu1 N1 84.0(5) . .
O24 Cu1 N1 84.0(5) 2_544 2_544
O24 Cu1 N1 96.0(5) . 2_544
N1 Cu1 N1 180.0 . 2_544
O1 Si1 O1 180.0 2 .
O1 Si1 O2 65.3(9) 2 2
O1 Si1 O2 114.7(9) . 2
O1 Si1 O2 114.6(9) 2 .
O1 Si1 O2 65.4(9) . .
O2 Si1 O2 180.0 2 .
O1 Si1 O3 68.0(8) 2 2
O1 Si1 O3 112.0(8) . 2
O2 Si1 O3 111.7(9) 2 2
O2 Si1 O3 68.3(9) . 2
O1 Si1 O3 112.0(8) 2 .
O1 Si1 O3 68.0(8) . .
O2 Si1 O3 68.3(9) 2 .
O2 Si1 O3 111.7(9) . .
O3 Si1 O3 180.0 2 .
O1 Si1 O4 73.0(8) 2 2
O1 Si1 O4 107.0(8) . 2
O2 Si1 O4 106.1(9) 2 2
O2 Si1 O4 73.9(9) . 2
O3 Si1 O4 104.5(8) 2 2
O3 Si1 O4 75.5(8) . 2
O1 Si1 O4 107.0(8) 2 .
O1 Si1 O4 73.0(8) . .
O2 Si1 O4 73.9(9) 2 .
O2 Si1 O4 106.1(9) . .
O3 Si1 O4 75.5(8) 2 .
O3 Si1 O4 104.5(8) . .
O4 Si1 O4 180.0 2 .
Si1 O1 O2 57.4(8) . .
Si1 O1 O3 57.3(8) . .
O2 O1 O3 98.8(12) . .
Si1 O1 Mo1 125.3(10) . .
O2 O1 Mo1 67.9(8) . .
O3 O1 Mo1 139.4(10) . .
Si1 O1 Mo2 123.5(9) . .
O2 O1 Mo2 135.0(11) . .
O3 O1 Mo2 66.2(7) . .
Mo1 O1 Mo2 95.5(6) . .
Si1 O1 Mo4 118.0(9) . .
O2 O1 Mo4 128.7(10) . .
O3 O1 Mo4 121.6(11) . .
Mo1 O1 Mo4 93.9(6) . .
Mo2 O1 Mo4 92.5(6) . .
Si1 O2 O1 57.2(9) . .
Si1 O2 O3 57.1(9) . 2
O1 O2 O3 98.5(13) . 2
Si1 O2 Mo1 126.7(10) . .
O1 O2 Mo1 69.5(8) . .
O3 O2 Mo1 136.8(10) 2 .
Si1 O2 Mo3 122.5(9) . .
O1 O2 Mo3 139.5(11) . .
O3 O2 Mo3 65.5(8) 2 .
Mo1 O2 Mo3 96.3(6) . .
Si1 O2 Mo5 117.5(9) . .
O1 O2 Mo5 125.0(11) . .
O3 O2 Mo5 124.8(10) 2 .
Mo1 O2 Mo5 93.1(6) . .
Mo3 O2 Mo5 92.3(7) . .
Si1 O3 O1 54.7(8) . .
Si1 O3 O2 54.7(8) . 2
O1 O3 O2 95.5(11) . 2
Si1 O3 Mo3 124.3(9) . 2
O1 O3 Mo3 137.3(11) . 2
O2 O3 Mo3 69.7(8) 2 2
Si1 O3 Mo2 123.8(9) . .
O1 O3 Mo2 69.2(7) . .
O2 O3 Mo2 141.9(11) 2 .
Mo3 O3 Mo2 97.6(7) 2 .
Si1 O3 Mo6 115.9(9) . .
O1 O3 Mo6 126.6(11) . .
O2 O3 Mo6 121.7(9) 2 .
Mo3 O3 Mo6 93.7(6) 2 .
Mo2 O3 Mo6 94.0(6) . .
Si1 O4 Mo4 120.5(8) . .
Si1 O4 Mo5 120.1(8) . 2
Mo4 O4 Mo5 98.2(6) . 2
Si1 O4 Mo6 118.7(8) . 2
Mo4 O4 Mo6 97.2(6) . 2
Mo5 O4 Mo6 97.0(6) 2 2
Mo1 O6 Mo4 135.4(8) . .
Mo2 O11 Mo6 138.4(8) . .
Mo6 O12 Mo4 136.2(12) . 2
Mo3 O13 Mo5 138.8(8) . .
Mo6 O14 Mo3 137.2(9) . 2
Mo2 O15 Mo1 136.4(11) . .
Mo5 O16 Mo1 136.7(9) . .
Mo3 O17 Mo2 132.4(12) . 2
Mo4 O19 Mo5 134.7(13) . 2
Mo1 O20 Mo3 136.3(10) . .
Mo4 O21 Mo2 136.3(8) . .
Mo5 O22 Mo6 133.7(10) . .
C6 O24 Cu1 114.5(10) . .
C1 N1 C5 118.4(14) . .
C1 N1 Cu1 129.5(12) . .
C5 N1 Cu1 112.1(10) . .
O23 C6 O24 125.7(16) . .
O23 C6 C5 119.0(15) . .
O24 C6 C5 115.3(14) . .
C16 C15 C14 120(2) . .
C15 C14 C13 123(2) . .
C11 N2 C7 114.7(19) . .
N1 C5 C4 121.9(15) . .
N1 C5 C6 114.1(14) . .
C4 C5 C6 123.8(15) . .
C14 C13 C12 118(2) . .
N3 C11 C10 119.0(19) . .
N3 C11 N2 118.0(19) . .
C10 C11 N2 123(2) . .
C3 C4 C5 116.8(16) . .
C2 C1 N1 123.6(18) . .
C9 C10 C11 121(2) . .
C15 C16 N4 123(2) . .
C15 C16 N5 117(2) . .
N4 C16 N5 120(2) . .
C12 N4 C16 120(2) . .
C4 C3 C2 119.5(16) . .
C10 C9 C8 120(3) . .
C1 C2 C3 119.6(17) . .
N4 C12 C13 116(2) . .
C9 C8 C7 120(2) . .
C8 C7 N2 121.7(19) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O5 1.665(11) .
Mo1 O20 1.837(13) .
Mo1 O6 1.880(13) .
Mo1 O16 1.908(12) .
Mo1 O15 1.972(13) .
Mo1 O2 2.346(17) .
Mo1 O1 2.372(18) .
Mo2 O10 1.665(11) .
Mo2 O15 1.832(14) .
Mo2 O11 1.851(13) .
Mo2 O21 1.919(13) .
Mo2 O17 1.992(15) 2
Mo2 O3 2.348(15) .
Mo2 O1 2.398(17) .
Mo3 O18 1.652(12) .
Mo3 O13 1.858(12) .
Mo3 O17 1.858(15) .
Mo3 O14 1.923(14) 2
Mo3 O20 1.977(12) .
Mo3 O3 2.334(19) 2
Mo3 O2 2.406(19) .
Mo4 O9 1.657(11) .
Mo4 O19 1.862(16) .
Mo4 O21 1.878(14) .
Mo4 O12 1.918(15) 2
Mo4 O6 1.951(15) .
Mo4 O4 2.316(16) .
Mo4 O1 2.478(17) .
Mo5 O7 1.633(13) .
Mo5 O16 1.880(14) .
Mo5 O22 1.914(16) .
Mo5 O13 1.925(13) .
Mo5 O19 1.952(15) 2
Mo5 O4 2.339(18) 2
Mo5 O2 2.501(19) .
Mo6 O8 1.653(12) .
Mo6 O14 1.866(16) .
Mo6 O12 1.868(15) .
Mo6 O22 1.921(17) .
Mo6 O11 1.944(14) .
Mo6 O4 2.369(16) 2
Mo6 O3 2.498(17) .
Cu1 O24 1.938(12) 2_544
Cu1 O24 1.938(12) .
Cu1 N1 1.945(13) .
Cu1 N1 1.945(13) 2_544
Si1 O1 1.586(17) 2
Si1 O1 1.586(17) .
Si1 O2 1.589(19) 2
Si1 O2 1.589(19) .
Si1 O3 1.635(19) 2
Si1 O3 1.635(19) .
Si1 O4 1.718(17) 2
Si1 O4 1.718(17) .
O1 O2 1.71(3) .
O1 O3 1.80(2) .
O2 O3 1.81(2) 2
O3 O2 1.81(2) 2
O3 Mo3 2.334(19) 2
O4 Mo5 2.339(18) 2
O4 Mo6 2.369(16) 2
O12 Mo4 1.918(15) 2
O14 Mo3 1.923(14) 2
O17 Mo2 1.992(15) 2
O19 Mo5 1.951(15) 2
O23 C6 1.22(2) .
O24 C6 1.289(19) .
N1 C1 1.35(2) .
N1 C5 1.36(2) .
C6 C5 1.49(2) .
C15 C16 1.28(3) .
C15 C14 1.33(3) .
C14 C13 1.35(3) .
N2 C11 1.37(3) .
N2 C7 1.42(3) .
C5 C4 1.41(2) .
C13 C12 1.47(4) .
C11 N3 1.33(3) .
C11 C10 1.35(3) .
C4 C3 1.40(3) .
C1 C2 1.31(3) .
C10 C9 1.34(3) .
C16 N4 1.39(3) .
C16 N5 1.42(3) .
N4 C12 1.36(3) .
C3 C2 1.41(3) .
C9 C8 1.36(3) .
C8 C7 1.37(4) .
